{'fraction_non_alphanumeric': 0.03370504949254479, 'fraction_numerical': 0.024025811301841875, 'mean_word_length': 4.831050228310502, 'pattern_counts': {'":': 0, '<': 1, '<?xml version=': 0, '>': 1, 'https://': 0, 'lorem ipsum': 0, 'www.': 0, 'xml': 0}, 'pii_count': 0, 'substrings_counts': 0, 'word_list_counts': {'cursed_substrings.json': 0, 'profanity_word_list.json': 0, 'sexual_word_list.json': 0, 'zh_pornsignals.json': 0}}
Enhanced charge separation in TiO2/nanocarbon hybrid photocatalysts through coupling with short carbon nanotubes

The interfacial contact between TiO2 and graphitic carbon in a hybrid composite plays a critical role in electron transfer behavior, and in turn, its photocatalytic efficiency. Herein, we report a new approach for improving the interfacial contact and delaying charge carrier recombination in the hybrid by wrapping short single-wall carbon nanotubes (SWCNTs) on TiO2 particles (100 nm) via a hydration-condensation technique. Short SWCNTs with an average length of 125 ± 90 nm were obtained from an ultrasonication-assisted cutting process of pristine SWCNTs (1–3 μm in length). In comparison to conventional TiO2–SWCNT composites synthesized from long SWCNTs (1.2 ± 0.7 μm), TiO2 wrapped with short SWCNTs showed longer lifetimes of photogenerated electrons and holes, as well as a superior photocatalytic activity in the gas-phase degradation of acetaldehyde. In addition, upon comparison with a TiO2–nanographene “quasi-core–shell” structure, TiO2-short SWCNT structures offer better electron-capturing efficiency and slightly higher photocatalytic performance, revealing the impact of the dimensions of graphitic structures on the interfacial transfer of electrons and light penetration to TiO2. The engineering of the TiO2–SWCNT structure is expected to benefit photocatalytic degradation of other volatile organic compounds, and provide alternative pathways to further improve the efficiency of other carbon-based photocatalysts.


Introduction
Rapid recombination of photogenerated electron-hole pairs is one of the major limitations of utilizing TiO 2 photocatalysts in applications such as water treatment, 1-3 air purication [4][5][6][7][8][9] bacterial and viral inactivation, 10,11 and self-cleaning glasses. [12][13][14] Most of the photogenerated electron-hole pairs recombine within 10 picoseconds (ps), which is very short compared to the 100 ps typically required for redox reactions. As a result, only a small portion ($10 percent) of the photogenerated charges, as revealed by time-resolved absorption spectroscopic studies, remain alive and able to participate in pollutant decomposition, resulting in limited photocatalytic activity. 15,16 A number of studies have shown that inhibition of charge recombination and remarkable enhancement in photocatalytic efficiency of TiO 2 can be achieved by coupling with carbon nanomaterials such as carbon nanotubes (CNTs), graphene, and fullerene. [17][18][19][20][21] The coupling leads to formation of a Schottky barrier, through which electrons efficiently travel from TiO 2 with a higher Fermi level to the carbon nanomaterial with a lower Fermi level until equilibrium is attained. 22,23 In addition, the high electron-storage capacity of the graphitic structure (one electron per 32 carbon atoms) can serve as electron reservoirs or sinks, decreasing the recombination probability of the photogenerated charges in the hybrid material and enhancing photocatalytic activity. 22 The improved charge separation in TiO 2 -nanocarbon hybrid structures depends largely on the quality of interfacial contact between TiO 2 and the graphitic structure, and the structural and surface properties of the hybrid components. 21,[24][25][26][27][28][29][30] A knowledge gap that still exists is how the graphitic structures and their geometries affect the coupling and interfacial contacts of the components in the hybrid. The rate of electron transport and subsequent separation of photogenerated charges in conventional TiO 2 -nanocarbon composites are still hampered by nonuniform coating or poor dispersion induced by TiO 2 aggregation on graphene sheets or CNT walls. Therefore, in light of the great promise shown by TiO 2 -nanocarbon hybrids in photocatalysis, research efforts have focused on tailoring the heterojunctions and schottky barriers to achieve efficient shuttling of electrons and promote electron-hole separation, as well as induce visible light excitation. It is well-established in the literature that charge recombination is inhibited on a variety of TiO 2 -CNT hybrids consisting of a thin, uniform TiO 2 layer on individual multi-walled CNTs (MWCNTs) or TiO 2 aggregates supported on CNTs. 29,[31][32][33][34] However, the trade-off relation between electron-hole concentration and separation efficiency in conventional TiO 2 -coated CNT composites remains a signicant impediment to maximizing the photocatalytic activity. 28 To this end, TiO 2 wrapped with graphene has been considered as an alternative to the TiO 2 /CNT core-shell (or TiO 2 -coated CNT) structure, as the concentration of photogenerated charges can be optimized without sacricing separation efficiency. 19,35 Signicant differences exist in hybrid structures formed with either CNTs or graphene. Graphene, a two-dimensional (2D) structure with several nanometers of width and high stacking tendency, can generate a "shell-like" structure consisting of several graphene layers on TiO 2 , preventing light penetration. 36,37 Another complication associated with graphene is the unavoidable electron scattering that may reduce the electron transport rate and promote charge recombination. 37 On the other hand, harnessing the one-dimensional (1D) single-wall CNT (SWCNT) structures in TiO 2 hybrids not only provides well-dened routes for electron transport, but also their small size compared to MWCNTs and graphene sheets provide a degree of freedom for optimizing charge separation without compromising light absorption. [38][39][40][41][42] A consensus from the aforementioned studies is that the structure of nanocarbons (i.e., the size of graphene or length of CNTs) is a crucial factor in controlling the quality of interfacial contact and subsequent charge separation. In particular, Kim et al. 36 revealed a superior photocatalytic activity for TiO 2 hybrids formed with nano-sized graphene (or nanographene) sheets in comparison to those formed with micro-sized graphene; the wrapping of nanographene on TiO 2 particles in the former hybrid maximized the interfacial contact between the components, resulting in superior charge separation and photocatalytic activity. Similarly, we hypothesize that cutting long SWCNTs into high populations of open-ended tubes with high degrees of functionalization and density of active sites, as well as short lengths that can effectively wrap a large TiO 2 particle ($100 nm), can lead to enhanced interactions with TiO 2 particles that will promote the photocatalytic process. Although many studies have investigated the inuence of coupling SWCNTs with TiO 2 , all reported works employed SWCNTs with lengths in the micrometer range.
In this study, we report for the rst time the wrapping of large TiO 2 particles ($100 nm) with short SWCNTs (125 AE 90 nm in length) obtained from an ultrasonication-assisted cutting process. The resulting TiO 2 -SWCNT hybrid photocatalyst exhibits enhanced interfacial contact and charge separation. The short, highly functionalized and dispersed SWCNTs, in the presence of TiO 2 , initiated formation of Ti-O-C bonds via intermolecular interactions, resulting in TiO 2 nanoparticles or nanoparticle aggregates that are partially wrapped by SWCNTs. In comparison to conventional TiO 2 -SWCNT composites synthesized using long SWCNTs (1.2 AE 0.7 mm), TiO 2 wrapped with short SWCNTs showed longer lifetimes of photogenerated electrons and holes, as well as a superior photocatalytic activity in the gas-phase degradation of acetaldehyde. In addition, upon comparison with a TiO 2 -nanographene "quasi-core-shell" structure, the novel TiO 2 -SWCNT composite offers superior electron-capturing efficiency and slightly higher photocatalytic performance, revealing the impact of the dimension of graphitic structures on the interfacial transfer of electrons and light penetration to TiO 2 .

Synthesis of TiO 2 -SWCNT composites
Puried SWCNTs (1-2 nm in diameter and 1-3 mm in length) were functionalized by reuxing with HNO 3 (70%) at 150 C for two hours. A known amount of functionalized SWCNTs were dispersed in ethanol and sonicated at 25 C for four hours to produce the short SWCNTs. Aer the sonication-assisted cutting process, the resulting suspension was allowed to settle for 15 minutes and the supernatant was slowly added to the TiO 2 -ethanol dispersion (50 mg in 50 mL ethanol) under sonication, followed by robust stirring overnight at pH ¼ 3.4. The sonicator (Branson, CPX5800H) operated at 100 W and 40 kHz. The TiO 2 particles (anatase, 99.9%, 100 nm) were purchased from US Research Nanomaterials, Inc. The TiO 2 -SWCNT hybrid synthesized from short SWCNTs (hereaer referred to as TiO 2short SWCNT) was collected by ltration using a membrane with average pore size of 0.2 mm and dried at 60 C. For TiO 2 -SWCNT hybrids synthesized from long SWCNTs, the same procedure was followed without subjecting the long SWCNTs to ultrasonication-assisted cutting; the resulting hybrid is here-aer referred to as TiO 2 -long SWCNT. Unless stated otherwise, the amount of SWCNTs used in the standard sample is 1 wt%.

Synthesis of TiO 2 -nanographene composites
The graphite powder was oxidized by the modied Hummer method. [43][44][45] The graphene oxide (GO) produced was treated with a mixture of HCl and KMnO 4 to produce the nanographene oxide. GO (0.05 g) was dispersed in 50 mL of concentrated HCl, and then 0.05 g of KMnO 4 was slowly added under robust stirring. Aer one hour of stirring at 40 C, the resulting slurry was cooled in an ice bath. Then, H 2 O 2 solution (5 mL H 2 O 2 and 95 mL distilled water) was slowly added with continued stirring for one hour, followed by sonication for 30 minutes to exfoliate the nanographene oxide. The nal product was collected by ltration using similar conditions in Section 2.1 and oven-dried at 60 C.
The TiO 2 -nanographene composite (0.7 wt% nanographene) was synthesized by dispersing a known amount of nanographene oxide in ethanol by sonication, and the resulting slurry was slowly added to the TiO 2 -ethanol dispersion (50 mg in 50 mL distilled water) under stirring at pH ¼ 3.5, followed by robust stirring overnight. The brownish powder obtained was transferred to a Teon-lined, hydrothermal synthesis autoclave reactor and heated at 120 C for 24 hours to reduce the nanographene oxide. The nal product (hereaer referred to as TiO 2nanographene) was washed repeatedly with 1 M HCl and distilled water, collected by ltration and dried at 60 C.

X-ray diffraction (XRD) patterns were collected on a Rigaku
Miniex II X-ray diffractometer with Cu Ka radiation (l ¼ 1.5418 A) at 40 kV and 40 mA. The Raman spectra were acquired via an iHR550 spectrometer with a laser excitation wavelength of 532 nm. Catalyst morphology was characterized by a eldemission scanning electron microscope (SEM, Hitachi S5200) equipped with energy-dispersive X-ray spectroscopy (EDS), and a transmission electron microscope (TEM, FEI Talos) operating at 200 kV. For TEM analysis, a small amount of the sample was dispersed in ethanol by sonication and dropped onto a copper microgrid coated with lacy carbon lm. X-ray photoelectron spectroscopic (XPS) measurements were collected via a Kratos Ultra XPS system at 1.0 Â 10 À9 Torr. A monochromatic Al Ka source (hn ¼ 1486.6 eV) operating at 10 mA and 12 keV (120 W) was used to collect the spectra. The effect of charging was reduced by a charge neutralizer. Survey spectra were collected at 160 eV pass energy with 1 eV step and 100 ms contact time. For the high-resolution scans, spectra were collected at 20 eV pass energy with 0.1 eV step and 100 ms contact time. The photoluminescence (PL) spectra were acquired via a spectraMax i3x multi-mode microplate reader over the range of 400-700 nm using an excitation wavelength of 360 nm.

Evaluation of photocatalytic activity
The photocatalytic activity was tested by measuring the change in concentration of gas phase acetaldehyde as a function of irradiation time. The photocatalyst (100 mg) was placed in a 750 mL borosilicate batch reactor surrounded by light sources (two 25 W Sylvania 21703 (356 nm) bulbs and two 13 W Repti-Sun 10.0 UV/B bulbs (280-320 nm) with intensity of 6.5 W m À2 ). One thousand ppmv of acetaldehyde gas was injected into the reactor via a syringe. Aer equilibrium between gaseous and adsorbed phases was attained, UV irradiation was started and the decrease in concentration was measured via an SRI 310C gas chromatograph equipped with a Restek silica gel column (8046-895, 6  length, 2 mm ID), on-column injection, and ame ionization detector (FID). According to the experimental data, acetaldehyde degradation by TiO 2 -short SWCNT, TiO 2 -long SWCNT and TiO 2 -nanographene tted to a pseudo rst-order reaction represented by eqn (1): where k is the apparent constant of reaction rate, c is the concentration of acetaldehyde and t is the reaction time.

Morphology, structure, composition, and interfacial properties
The SEM image in Fig. 1a reveals TiO 2 particles are partially wrapped by short SWCNTs (TiO 2 -short SWCNT), a phenomenon that occurs uniformly over a large area on TiO 2 particles. EDS mapping of TiO 2 -short SWCNT (Fig. 1b) reveals the co-existence  (002) and (100) crystal planes of SWCNTs, were not detected in TiO 2 -short SWCNT, due to the low SWCNT concentration (1 wt%). However, the addition of SWCNTs slightly reduced the relative intensity of TiO 2 peaks, an observation consistent with other studies. 46,47 Raman spectra (Fig. 2b) show the characteristic peaks of anatase TiO 2 at 397, 515, and 639 cm À1 . 48 The characteristic anatase peaks (B 1g , A 1g + B 1g , and E g ) were observed in TiO 2 -short SWCNT, accompanied by the disordered carbon-induced D-band at 1350 cm À1 , and the G-band at 1583 cm À1 that represents sp 2 carbon from SWCNTs. The slight shi in anatase modes observed in the Raman and XRD spectra generally correlates with the external perturbation by SWCNTs and the corresponding substitution of Ti 4+ by C atoms, resulting in the formation of Ti-O-C bonds in the TiO 2 lattice. [49][50][51][52] However, band gaps of TiO 2 and TiO 2 -short SWCNT (calculated from UV-Vis spectra in Fig. S4 †) are 3.22 and 3.19 eV, respectively, suggesting low-carbon doping in the composite.
An XPS survey spectrum of TiO 2 -short SWCNT conrms the presence of Ti, O, and C (Fig. 3a). The high-resolution XPS spectrum of Ti 2p (Fig. 3b) shows two peaks located at 459.5 and 465.2 eV attributed to Ti 2p 3/2 and Ti 2p 1/2 , respectively, which are typical binding energies of the Ti 4+ valance state. 53 The O 1s spectrum, shown in Fig. 3c, is tted with three peak components. The component at 530.7 eV corresponds to Ti-O-Ti, while the peak at 531.6 eV is attributed to C]O or C-OH. 53 The peak at 532.8 eV is ascribed to Ti-O-C, and is an indication of the covalent interaction between TiO 2 and SWCNTs. 54 Based on density functional theory calculations, 55 Ti-O-C bonds facilitate charge carrier separation due to their higher electrostatic density in comparison to the non-covalent interaction. As a consequence, the charge redistribution map predicts a higher rate of electron transport. The C 1s region, shown in Fig. 3d, is  tted with four peak components. The peak at 284.5 eV is assigned to sp 2 carbon, while the peaks at 285.7, 287.7, and 289.8 eV are assigned to functional groups linked to the carbon atoms including C-O/C-O-Ti, C]O, and O-C]O, respectively. 54,56 The various oxygen functional groups generate anchors for direct linking with TiO 2 . The absence of the Ti-C peak, typically located at 281 eV, 57 conrms our claim regarding the absence of signicant carbon doping in the composite.

Photocatalytic degradation of gaseous acetaldehyde by TiO 2 -SWCNT hybrids
To evaluate the photocatalytic activity of TiO 2 wrapped with SWCNTs, the degradation of acetaldehyde was conducted under UV light. Fig. 4a shows the effect of SWCNT amount in the hybrid structure on photocatalytic activity expressed in terms of normalized acetaldehyde concentration aer 60 minutes. Coupling of short SWCNTs with TiO 2 markedly improves degradation of acetaldehyde. The photocatalytic degradation activity is sensitive to the amount of SWCNTs in the composite; our ndings revealed the optimum amount to be 1 wt%. A schematic illustration of the proposed mechanism for photocatalytic degradation of gaseous acetaldehyde on TiO 2 -short SWCNT hybrid is depicted in Fig. 4b. Upon light illumination, photo-induced electron-hole pairs are produced by TiO 2 (hv (<350 nm) / e À CB+SWCNTs + h + ); the electrons are promoted to the conduction band leaving holes in the valance band. 58 The CB position of anatase is $4.21 eV using vacuum level (AVS) (À0.4 eV relative to reversible hydrogen electrode (RHE)), with a bandgap of about 3.2 eV. On the other hand, the work function of a SWCNT is known to be $À4.8 eV (AVS) (approximately 0.2 relative to RHE). 59 Since the work function of SWCNTs is lower than the conduction band of TiO 2 , SWCNTs can act as electron sinks whereby a fraction of the photoelectrons ow to them. 41,59 The holes in the valence band react with water molecules to generate hydroxyl radicals (cOH) (H 2 O + h + / cOH + H + ), while the photoexcited electrons in SWCNTs and in the conduction band of TiO 2 react with O 2 to produce superoxide radicals (cO 2 À ) (O 2 + e À CB+SWCNTs ¼> cO 2 À ). The active radicals initiate decomposition of adsorbed gaseous acetaldehyde via two reaction pathways. cOH and cO 2 À could oxidize a portion of  Fig. 4c, the relevant potential level of the acceptor species is located below the CB potential of TiO 2 . On the other hand, the potential level of the donor species is above the valence band position of TiO 2 , validating the generation of active radicals responsible for the degradation of gaseous acetaldehyde. [63][64][65][66][67][68][69] It is well known the photogenerated electron-hole pair participates in redox reactions on the catalyst surface to initiate degradation of adsorbed pollutant; however, the process is limited by rapid recombination of electrons and holes. As depicted in Fig. 4b, one of the roles of SWCNTs in TiO 2 -CNT composites is to inhibit electron-hole recombination. 15, 16 An increase in the amount of SWCNTs in the hybrid composite beyond 1 wt% has a negative effect on the photocatalytic performance, which we attribute to SWCNT aggregation and generation of large SWCNT bundles. Hsu and coworkers [70][71][72][73][74][75] have provided further mechanistic insight into the effect of nanocarbon loading on photocatalytic performance. The overall charge separation efficiency in nanocarbon-semiconductor hybrids can be sacriced when the amount of the electron sink (metal or nanocarbon) exceeds the optimum value. The observed trend in activity for the different TiO 2 -SWCNT ratios in our study is consistent with the results from these studies and can also be rationalized by the so called later-emerging electron-hole recombination that is induced across the interface. The formation of large-diameter bundles indicates SWCNTs at high concentration tend to interact with each other via Van der Waals forces rather than with TiO 2 . As a consequence, the quality of the interfacial contact (or degree of interaction) between TiO 2 and SWCNTs is reduced. In addition, the coverage of thick SWCNT bundles on TiO 2 particles has the potential of signicantly decreasing light penetration to TiO 2 , thus reducing photoactivity as observed in other studies that involve wrapping of graphene on TiO 2 or coupling graphene quantum dots with TiO 2 . 41,76 Despite the decrease in photocatalytic activity upon SWCNT aggregation, the observed performance is still higher than pristine TiO 2 , indicating photon permeation is not completely blocked and the benecial role of SWCNTs in photocatalytic enhancement, via charge separation, may still be partially maintained.

Effect of SWCNT length and graphitic dimensions on interfacial contact, charge separation, and photocatalytic activity of the hybrids
To probe the inuence of SWCNT length on the interfacial contact and subsequent photocatalytic performance of TiO 2 -SWCNT hybrids, we synthesized another composite with long SWCNTs (TiO 2 -long SWCNT) using the same concentration of SWCNTs, but without subjecting the sample to the ultrasonication cutting step. Representative TEM images for long SWCNTs and short SWCNTs used for coupling with TiO 2 are presented in Fig. S5 † with corresponding box plots in Fig. 5 showing their length distributions; each box plot consists of 12 measurements of nanotubes from TEM images. The average length of short SWCNTs is 125 AE 90 nm while that of long SWCNTs is 1.2 AE 0.67 mm. The results clearly demonstrate the shear force generated by ultrasonication results in SWCNTs that are signicantly shorter than those processed without ultrasonication. The use of ultrasonication as a nondestructive technique for cutting nanotubes is well established in processing nanomaterials. Shuba et al. 77 showed that ultrasonication yields SWCNTs with low side-wall degradation and preserves the electronic properties of the nanotubes. Note that for SWCNTs to efficiently play the intended role of "electron sink" in hybrid structures during photocatalysis, preserving their structural integrity and exceptional electronic properties is critically important.
The Raman spectra of pristine SWCNTs, short SWCNTs, and long SWCNTs in Fig. 6 provide further insight into the effect of the processing approach on the structure of SWCNTs. The ratio of G-to D-band intensities (I G /I D ) from the Raman spectra, widely considered a quality or graphitization index for carbonbased materials, 78-80 is 13.9 for pristine SWCNTs and decreases to 3.3 and 3.6 aer acid treatment for long SWCNTs and short SWCNTs, respectively, due to the functionalization of SWCNTs. The I G /I D ratios for short and long SWCNTs are about the same, which indicates that the ultrasonication process did not degrade the nanotubes. As observed previously in Fig. 2b, the TiO 2 -SWCNT composite exhibited a slight decrease in I G /I D , suggesting the increase in defect aer the coupling of TiO 2 and SWCNTs, 49 probably due to the low substitution of Ti 4+ by carbon atoms. In addition, the characteristic phonon mode in SWCNTs occurring in the low frequency region (zoomed in the insets), the radial breathing mode (RBM), is clearly observed in pristine and processed SWCNTs. In fact, the same RBM peaks for pristine SWCNTs at $150 and 260 cm À1 are observed for long SWCNTs and short SWCNTs. This provides further evidence that the ultrasonication process did not destroy the nanotubes.
Next, we investigate the effect of SWCNT length and nanocarbon dimension on interfacial contact, charge separation, and photocatalytic activity of the hybrids. Electron microscopic images of the resulting hybrids formed with short SWCNTs, long SWCNTs and nanographene, along with corresponding EDS mapping for TiO 2 -nanographene, are shown in Fig. 7. The EDS mapping of TiO 2 -nanographene reveal a highly uniform distribution of titanium, carbon, and oxygen as observed for TiO 2 -short SWCNT (Fig. 1b). In contrast to TiO 2 -short SWCNT (Fig. 7a), bundles of large-diameter SWCNTs are apparent in TiO 2 -long SWCNT composites (Fig. 7b), with severe particle aggregation as shown in Fig. S6. † These observations give credence to the assumption that ultrasonication not only reduces the length of SWCNTs, but also facilitates debundling of SWCNTs. Morphological characterization of micron-sized  graphene, exfoliated nanographene, and non-exfoliated nanographene are summarized in Fig. S7. † The average size the nanographene, as determined from TEM analysis and shown on the box plot (Fig. S7 †), is $125 AE 93 nm.
Photocatalytic degradation of acetaldehyde by TiO 2 , TiO 2long SWCNT, TiO 2 -nanographene, and TiO 2 -short SWCNT, is shown in Fig. 8a along with the PL spectra of the photocatalysts in Fig. 8b. As depicted in Fig. 8a, TiO 2 -short SWCNT shows the highest performance; the rate constant of TiO 2 -short SWCNT is 0.015 min À1 , while others are given as follows: pristine TiO 2 (k ¼ 0.0073 min À1 ), TiO 2 -long SWCNT (k ¼ 0.0107 min À1 ), and TiO 2nanographene (k ¼ 0.0125 min À1 ). TiO 2 -short SWCNT showed better performance compared with TiO 2 -nanographene, even though the quality of interfacial contact in the two heterostructures is somewhat similar, as evidenced by EDS mapping that reveals a highly uniform distribution of nanographene on TiO 2 particles  over a large area (Fig. 7d). The PL spectra (Fig. 8b) show lifetimes of charges on TiO 2 coupled with short SWCNTs are longer than TiO 2 coupled with nanographene, which explains the different photocatalytic activities observed as evidenced by their rate constants.

Discussion
Based on our results, we present a schematic illustration of the interfacial contact between nanocarbon (short SWCNTs, long SWCNTs or nanographene) and TiO 2 , as well as the charge carrier movement in the hybrids in Fig. 7. We rationalize the superior performance of TiO 2 -short SWCNT to be due to the inhibition of charge recombination in the composite, which can be achieved in two ways. First, the increase in the number of interfacial contacts between each individual TiO 2 and short SWCNTs provides more channels for electron transport that inhibits charge recombination. The short and well-exfoliated SWCNTs can have lower bending stiffness compared to the long and non-exfoliated SWCNTs. It has been shown that bending stiffness of SWCNTs is directly proportional to SWCNT diameter; 81 therefore, we expect large-diameter SWCNT bundles to have larger persistence length compared to exfoliated SWCNTs (or small-diameter SWCNT bundles). Hence, short SWCNTs efficiently wrap a TiO 2 particle (Fig. 9a). Consequently, a large fraction of TiO 2 nanoparticles are in direct contact with short SWCNTs. In contrast, only a small fraction of TiO 2 nanoparticles are in direct contact with the long SWCNTs (Fig.  9b). Second, the improved SWCNT debundling ensures a uniform distribution of SWCNTs over a large area on the TiO 2 surface, and hence, the shuttling of electrons across the interface for enhanced charge separation is not restricted to a small portion of the composite as in the case of TiO 2 -long SWCNT hybrids. To test the above hypotheses, PL data presented in Fig. 8b provide valuable insight. In comparison to pristine TiO 2 , uorescence quenching was observed in the TiO 2 -SWCNT hybrid structures, conrming the transfer of electrons from TiO 2 to SWCNTs delayed charge recombination. It is clear from the PL results that the intensity of TiO 2 -short SWCNT hybrids is lower than that of TiO 2 -long SWCNT hybrids, and is substantially lower than pristine TiO 2 , conrming the efficient charge separation occurring in TiO 2 -short SWCNT hybrids.
To rationalize the role of short SWCNTs (or oxygencontaining functionalities), we have to consider the synthesis steps, and in particular, the zeta potentials of SWCNTs and TiO 2 particles in ethanol under the pH used. Factors such as type of solvent and pH of mixture can alter the surface charge of nanostructures. In our case, acid treatment lowers the zeta potential of SWCNTs due to the formation of oxygen functionalities as shown by Liu et al. 82 These functional groups on the surface and tips of short SWCNTs imparts a strong negative charge and make them more easily dispersed. The negatively charged groups provide a strong electrostatic attraction toward positively charged species. Conversely, at low pH or high hydrogen ion activity, the surface of TiO 2 acquires a positive charge due to the high zeta potential. In fact, Widegren and Bergström 83 showed that the addition of a relatively small amount of acid or base is capable of introducing a relatively strong charge on TiO 2 particles. In our synthesis experiment, TiO 2 particles and functionalized SWCNTs were dispersed in ethanol at pH ¼ 3.5 which creates an environment with a high hydrogen activity and a strong positive charge on TiO 2 . The strong positively charged TiO 2 particles and negatively charged functionalized SWCNTs interact strongly via electrostatic attraction to form the hybrid structures with enhanced interfacial contact. In addition, opened and unblocked CNTs signicantly increase the density of adsorption or anchoring sites. 84 Cutting of long SWCNTs increases the number of open ends, and therefore, the short SWCNTs provide more "handles" or anchoring sites for interactions with TiO 2 than long SWCNTs.
The dimension of the graphitic structure is another important factor that can affect charge separation. To understand the role of the dimension of the graphitic structure in the composite, we compared the performance of TiO 2 quasiwrapped by 1D SWCNTs (TiO 2 -short SWCNT) with the quasiwrapped by 2D nanographene (TiO 2 -nanographene). The synthesis of the quasi-core-shell structure is adapted from a technique proposed by Kim et al. 36 We hypothesize that random pathways in 2D graphene can signicantly reduce the electron transport rate or may lead to electron escape from the graphene sheet (as schematically depicted in Fig. 9c), and thus promote charge carrier recombination. In contrast, the 1D SWCNTs offer efficient and short pathways for the transfer of vectorial electrons and, hence, enhanced charge separation. In addition, nanographene has a high stacking tendency and even aer exfoliation, the number of layers cannot be easily controlled. During TEM analysis, we observed several TiO 2 nanoparticles with thick graphitic shells, considerably thicker than SWCNT bundles (see Fig. 7c and e). This means signicant portion of incident light is hindered from reaching TiO 2 in a typical core-shell structure for TiO 2 -nanographene. On the other hand, SWCNTs, even in the case of bundles, due to their one-dimensional structure and small diameters, do not completely block light permeation to TiO 2 , as shown earlier for hybrid structures synthesized using high SWCNT concentrations. Nevertheless, coupling short SWCNTs or nanographene signicantly improved electron-hole separation and photoreactivity of TiO 2 ; the photoexcited electrons in the TiO 2 core are efficiently transported into the nanocarbon due to the strong interfacial contact between the hybrid components.

Conclusions
TiO 2 nanoparticles quasi-wrapped with short SWCNTs were successfully fabricated via an approach that involves the interaction between TiO 2 and short SWCNTs in ethanol as a solvent. The presence of short SWCNTs resulted in enhanced photocatalytic activity and efficient charge separation. The improved interfacial contact, veried by electron microscopy, prolonged the lifetime of an electron-hole pair on TiO 2 as demonstrated by photoluminescence spectroscopy. Unlike hybrid structures with long SWCNTs, higher photocatalytic performance in gas-phase degradation of acetaldehyde was achieved with TiO 2 -short SWCNT hybrids, conrming use of short SWCNTs in coupling with TiO 2 as a better alternative. Investigations into the effect of nanocarbon dimensions on charge separation revealed TiO 2short SWCNT hybrids have slightly higher photocatalytic activity than TiO 2 -nanographene. We attribute the performance to electron scattering in 2D-nanographene, which may affect electron transport through the interface. The high stacking tendency of nanographene may form a thick graphitic layer on TiO 2 that could hinder UV light penetration. Overall, this study provides rational new guidelines for maximizing electron-hole separation in TiO 2 -nanocarbon hybrids for improved photocatalytic performance.

Conflicts of interest
There are no conicts to declare.